J Adv Prosthodont 2015;7:454-9
Effect of different veneering techniques on the fracture strength of metal and zirconia frameworks Ayse Gozde Turk1, Mubin Ulusoy1, Mert Yuce2, Hakan Akin3* Department of Prosthodontics, Faculty of Dentistry, University of Ege, Izmir, Turkey Private practice, Izmir, Turkey 3 Department of Prosthodontics, Faculty of Dentistry, Cumhuriyet University, Sivas, Turkey 1 2
PURPOSE. To determine whether the fracture strengths and failure types differed between metal and zirconia frameworks veneered with pressable or layering ceramics. MATERIALS AND METHODS. A phantom molar tooth was prepared and duplicated in 40 cobalt-chromium abutments. Twenty metal (IPS d.SIGN 15, Ivoclar, Vivadent, Schaan, Liechtenstein) and 20 zirconia (IPS e.max ZirCAD, Ivoclar) frameworks were fabricated on the abutments. Each framework group was randomly divided into 2 subgroups according to the veneering material: pressable and layering ceramics (n=10). Forty molar crowns were fabricated, cemented onto the corresponding abutments and then thermocycled (5-55°C, 10,000 cycles). A load was applied in a universal testing machine until a fracture occurred on the crowns. In addition, failure types were examined using a stereomicroscope. Fracture load data were analyzed using one-way ANOVA and Tukey HSD post-hoc tests at a significance level of 0.05. RESULTS. The highest strength value was seen in metal-pressable (MP) group, whereas zirconia-pressable (ZP) group exhibited the lowest one. Moreover, group MP showed significantly higher fracture loads than group ZP (P=.015) and zirconia-layering (ZL) (P=.038) group. No significant difference in fracture strength was detected between groups MP and ML, and groups ZP and ZL (P>.05). Predominant fracture types were cohesive for metal groups and adhesive for zirconia groups. CONCLUSION. Fracture strength of a restoration with a metal or a zirconia framework was independent of the veneering techniques. However, the pressing technique over metal frameworks resisted significantly higher fracture loads than zirconia frameworks. [ J Adv Prosthodont 2015;7:454-9] KEY WORDS: Dental porcelain; Zirconia; Crowns; Compressive strength
INTRODUCTION During the past 40 years, the porcelain fused to metal technique has proven to be a reliable treatment option for fixed partial dentures and still represents the gold standard. 1 Corresponding author: Hakan Akin Department of Prosthodontics, Faculty of Dentistry, Cumhuriyet University, Yeni Şehir Mah. Kayseri Cad. Dış Kapı No:69, 58140 Sivas, Turkey Tel. 903462191010-2794: e-mail, [email protected]
Received May 14, 2015 / Last Revision September 2, 2015 / Accepted October 20, 2015 © 2015 The Korean Academy of Prosthodontics This is an Open Access article distributed under the terms of the Creative Commons Attribution Non-Commercial License (http://creativecommons. org/licenses/by-nc/3.0) which permits unrestricted non-commercial use, distribution, and reproduction in any medium, provided the original work is properly cited.
However, due to the rising interest in esthetic dentistry, zirconia which is a computer-aided design/computer aided manufacturing (CAD/CAM) bilayer restoration have gained popularity with its superior mechanical properties such as high flexural strength (700 - 1,200 MPa), fracture toughness (7 - 10 MPa·m1/2), hardness, translucency,2 chemical stability,3-5 biocompatibility, and favorable optical properties.6 Metal or zirconia core materials must be covered with a feldspathic veneering ceramics to establish an optimum esthetic outcome especially color and translucency.7,8 Different techniques, including layering and pressing techniques, can be performed for veneering ceramic on core materials.9 In the layering technique, the porcelain powder is mixed with modeling liquid, and the mixture is brush-applied on the core (metal or fully-sintered zirconia) larger than the final dimensions to compensate for the shrinkage of the veneering ceramic.8 Furthermore, multiple applications and firings pISSN 2005-7806, eISSN 2005-7814
Effect of different veneering techniques on the fracture strength of metal and zirconia frameworks
(minimal three firing cycles, namely dentin, enamel and glaze firings), which are carried out by the skillful dental technician, are required.10 On the other hand, in the pressing technique, prior to investing, a final contour anatomical waxing is prepared on a core. After elimination of the wax in an oven, ceramics are heat-pressed into the mold and to the core.8 This technique has some advantages on the layering technique with its speed, accuracy and stability. Moreover, the core and wax pattern complex can be tried in the mouth before final laboratory processes of the pressing ceramic.9,11 Additionally, the shrinkage related problems as well as consequences of possible sintering procedures are eliminated.8 For the zirconia-based ceramic restorations, delamination of the veneering porcelain from the core structure (chipping of the veneering ceramic) is a major failure mode.4,12 Ceramic structures tend to fail because of surface tension, where cracks and flaws propagate by slow crack growth leading to the failure. The flaw size, number and distribution can be related to the material, or be affected by the fabrication process. 13 Chipping can be attributed to potential flaws and artifacts generated during the veneering technique.14 As the pressing technique is a more controlled procedure, fewer flaws and better strength properties are expected than the layering technique.15 In literature, very limited data has been reported about evaluating pressable ceramics on metal and zirconia core materials and comparing them with layering ones.8,16,17 Thus, the aim of this in vitro study was to investigate the load bearing capacities of pressable and layering ceramics to the corresponding metal and zirconia frameworks. The hypothesis was that the fracture strength of metal or zirconia based ceramic restoration is independent of the veneering techniques.
MATERIALS AND METHODS In this in vitro study, base metal alloy and zirconia were used as core materials; pressing and layering techniques were performed as veneering materials to produce posterior crowns. A phantom mandibular molar tooth (Frasaco GmbH, Tettnang, Germany) was prepared with a 1 mm circumferential chamfer preparation and tapered angle of 8˚, using a surveyor (F1, DeguDent, Hanau, Germany). Forty impressions (Affinis Precious, Coltene/Whaledent, Altstätten, Switzerland) were taken and the prepared tooth was duplicated in 40 cobalt-chromium alloy dies (Remanium 2000, Dentaurum, Ispringen, Germany) in order to standardize the frameworks. Metal dies were randomly divided into 2 groups according to the framework types: metal and zirconia (n = 20). Twenty wax patterns were built on dies and 20 metal frameworks (IPS d.SIGN 15, Ivoclar Vivadent, Schaan, Liechtenstein) with a thickness of 0.5 mm were fabricated with lost-wax technique. The metal frameworks were randomly divided into 2 subgroups and coded by veneering process, layering (ML) and pressing (MP) groups (n = 10). In the ML group, two layers of opaque (IPS InLine
Opaquer, Ivoclar Vivadent) was applied to the metal surface and fired under vacuum in a calibrated porcelain oven (Programat 500, Ivoclar Vivadent) to 930°C. Then, leucite based body porcelain (IPS InLine, Ivoclar Vivadent) was vibrated and condensed to produce minimal shrinkage during processing. The crown was completed with a buccolingual width of 8 mm, a mesiodistal width of 10 mm, and an occlusal thickness of 2 mm after 3 firing cycles under vacuum at 910°C, including glaze firing. A silicone index was made from the outer surface of the first finished crown. This index was then used by the dental technician to fabricate all crowns. In the MP group, two layers of opaque (IPS InLine Opaquer, Ivoclar Vivadent) was applied and fired. Subsequently, a pressable ceramic wax-up was applied using an ash-free wax (XP Dent Corp., Miami, FL, USA) with the silicone index. The metal-opaque-wax specimen was sprued and invested (IPS PressVEST Speed Investment, Ivoclar Vivadent). Wax elimination was performed according to the manufacturer’s instructions. Ingots (IPS InLine PoM, Ivoclar Vivadent) were placed in the pressing furnace (EP600 Combi, Ivoclar Vivadent) and pressed at 940°C. The hot investment ring was left to cool to room temperature. Then the specimens were divested, finished, and glazed at 800°C (Fig. 1). The metal dies (n = 20) were scanned and 20 zirconia copings with a thickness of 0.5 mm were produced by a CAD/ CAM system (InLab, Sirona Dental Company, Bensheim, Germany) using pre-sintered zirconia (IPS e.max ZirCAD, Ivoclar Vivadent), then sintered in a furnace (Sintramat, Ivoclar Vivadent). A liner (ZirLiner, Ivoclar Vivadent) was applied on the zirconia frameworks and fired at 960°C according to the manufacturer suggestion. The frameworks were divided into 2 groups: 10 were veneered with layering technique (ZL) and 10 were veneered with pressing technique (ZP). In the ZL, a glass-ceramic material (IPS e.max Ceram, Ivoclar Vivadent) was used to build up zirconia frameworks with the previously taken silicone index. The final shapes of the crowns were performed with 2 firing processes (dentin and enamel firing) at 750°C and for a final firing, the
Fig. 1. Metal and zirconia based ceramic specimens before cementation. The Journal of Advanced Prosthodontics
J Adv Prosthodont 2015;7:454-9
crowns were glazed at 725°C according to the manufacturer’s instructions. In the ZP, the silicone index was used to duplicate the wax-up veneering part of the zirconia frameworks. A sprue was attached to the wax-framework complex and invested. The wax was eliminated in the oven and the pressable fluorapatite glass ceramic ingots (IPS e.max ZirPress, Ivoclar Vivadent) were pressed into the pressing ring (EP 600, Ivoclar, Vivadent) at 910°C then glazed at 770°C. All veneer build-up and firing procedures were performed according to the manufacturer’s instructions by the same dental technician (Fig. 1). The crowns were cemented (Panavia F 2.0, Kuraray Medical, Okayama, Japan) onto the corresponding metal dies according to the manufacturer’s instructions. The cemented crowns were then underwent thermocycling (5-55°C, 10,000 cycles) to simulate aging. Afterwards, they were p l a c e d i n a u n ive r s a l t e s t i n g m a ch i n e ( S h i m a d z u Corperation, Tokyo, Japan) (Fig. 2). The load was applied with a 6 mm diameter stainless steel ball at a crosshead speed of 0.5 mm/min until fracture of the crown occured. To avoid high stress concentration on the veneering material, a 1 mm thin piece of ethylenvinylacetat foil (Bioplast, Scheu Dental, Iserlohn, Germany) was placed on the occlusal surfaces. The load at fracture was determined by the first discontinuity in the load, whether it was an early crack or a catastrophic failure. After testing, all fractured specimens were examined under a stereomicroscope (Leica DFC295, Leica, Bensheim, Germany) at ×10 magnification by one operator to detemine the failure types. The loads at fracture were registered and the SPSS program (version 13.0, SPSS Inc., Chicago, IL, USA) was used for statistical analysis. Independent samples t-test was used for analysis of the effects of framework material and veneering technique, then followed by one-way ANOVA and Tukey HSD post hoc test to make comparisons among the groups. P was set as 0.05 in all analyses.
Fig. 2. Load was applied on each crown using a spherical indenter with an ethylen-vinyl acetate foil.
RESULTS The mean fracture loads were presented in Table 1. Oneway ANOVA showed statistically significant difference between the groups (P = .01). The highest fracture load was detected in group MP and the lower one seen in group ZP. In addition, analysis of data revealed that the mean fracture load of group MP was significantly higher than group ZL (P = .038) and group ZP (P = .015). There were no significant differences between other groups: MP and ML, ZP and ZL, ML and ZP, ML and ZL (P > .05) (Table 1). In metal groups, the fracture types were predominantly cohesive within frameworks (Fig. 3) (except one adhesive fracture for the pressing group) but there was no total fracture of the framework. In zirconia groups, the fractures were adhesive or cohesive within the veneering ceramics (Fig. 4) (7 adhesive, 3 cohesive for the layering group; 8 adhesive, 2 cohesive for the pressing group) (Table 2).
Table 1. Mean fracture loads (N) and standard deviations (SD) and statistical analyses Mean (SD) (N)
p2-3=0.038* p2-4=0.015* p3-4=0.952